- Nano Express
- Open Access
Nanoscale Inhomogeneities Mapping in Ga-Modified Arsenic Selenide Glasses
Nanoscale Research Letters volume 12, Article number: 88 (2017)
Nanoscale inhomogeneities mapping in Ga-modified As2Se3 glass was utilized exploring possibilities of nanoindentation technique using a Berkovitch-type diamond tip. Structural inhomogeneities were detected in Gax(As0.40Se0.60)100−x alloys with more than 3 at.% of Ga. The appeared Ga2Se3 nanocrystallites were visualized in Ga-modified arsenic selenide glasses using scanning and transmission electron microscopy. The Ga additions are shown to increase nanohardness and Young’s modulus, this effect attaining an obvious bifurcation trend in crystallization-decomposed Ga5(As0.40Se0.60)95 alloy.
Chalcogenide glasses (ChG), e.g., chemical compounds of chalcogens (S, Se, or Te, but not O) with some elements from IV–V groups of the Periodic table (such as As, Sb, Ge, Bi) prepared by rapid quenching from a melt have found widespread application in modern photonics and optoelectronics because of their superior transmittance in IR domain ranged from visible to nearly 20–25 μm [1–3]. This important class of disordered materials sometimes distinguished as functional media of chalcogenide photonics  can be well-represented by several canonical systems (model glass-formers), where arsenic triselenide As2Se3 (i.e., As40Se60 as classified in specialized glass-chemistry terminology) in the form of melt-quenched bulky rods, drawn fibers, deposited, or sputtered thin films, etc. plays a crucial role [1–4].
For a long time, these As2Se3-type ChG have been preferentially used as passive photonics elements, only transmitting light from one point to another. In the last decades, it was shown that due to purposeful rare-earth (RE) doping, these glasses could be also employed for a number of very important active device applications [3, 4]. In this case, the mid-IR light can be initiated by emission of excited RE ions (such as Pr3+, Er3+, Dy3+, Tb3+) on different wavelengths, thus creating the remote sources of light [5–8]. From purely implementation point, it is important to achieve a high enough concentration of RE ions in ChG. One of best solutions relies on introducing Ga (or In) into ChG matrix, permitting dissolution of higher ratio of RE dopants [8–13]. However, the Ga additions may essentially restrict glass-forming ability in many ChG systems [8, 11, 13–15] provoking parasitic devitrification processes at a nanoscale through phase separation, crystallite nucleation, growth, and extraction (uncontrolled spontaneous crystallization). Thus, it was shown, that in case of glassy As2Se3 it is not possible to introduce more than 3 at.% of Ga without such intrinsic structural decomposition, which essentially influences the ChG functionality [8, 12, 14].
It is understandable that reliable experimental monitoring of such nanoscale inhomogeneities in Ga-modified ChG is very important problem in the engineering of modern chalcogenide photonics. In this work, such methodology based on nanoindentation mapping supported by a number of electron microscopy visualization techniques will be examined at the example of Ga-modified As2Se3 glasses.
Conventional melt-quenching technique was employed to prepare Gax(As0.40Se0.60)100−x (x = 0−5) samples using high purity commercial elemental precursors of Ga (7N), As (5N), and Se (5N) [12–14]. The As and Se were specially purified by distillation with low evaporation rate to remove impurities such as oxygen, water, silica, and carbon. The appropriate amounts of initial elements with total weight of 30 g were introduced into a silica tube of 10 mm in diameter. The ampoule was sealed under vacuum and heated up to 900 °C in a rocking furnace for 10 h followed by quenching into water from 700 °C. After quenching, the samples were swiftly moved to preheated furnace for annealing for 5 h at the temperature of 10 °C below glass transition temperature (to remove mechanical strains induced by fast quenching). The obtained rods were cut into disks of ~2 mm in thickness and polished to high optical quality.
The method of nanoindentation mapping  was probed as a tool to disclose possible nanoscale inhomogeneities caused by Ga additions in As40Se60 glass. The values of nanohardness (NHD) and reduced elastic modulus (the Young’s modulus E) were detected with a help of CSM nanoindentation instrument (CSM Instruments SA, Peseux, Switzerland) equipped with a pyramidal Berkovitch-type diamond tip with a radius of about 100 nm employing the known Oliver-Pharr method  for data analysis. The standard samples of fused silica with elastic modulus of 73 GPa and Poisson’s ratio of 0.17 were used for indenter calibration allowing reliable load and displacement resolution at the level of 10 nN and 0.1 nm, respectively. The trapezoidal load-displacement curves (as those shown in Fig. 1 for As40Se60 and Ga3(As0.40Se0.60)97 glasses) were detected simultaneously for maximal load of 10 mN and loading-unloading rate of 20 mN/min, the dwell time at maximal loading being set to 15 s.
The tested sample’s surface was scanned within a uniform grid of nanoindentation series (incl. 7–10 separate measurements). Such arranged experimental measuring protocol allows a quite acceptable locality of each measuring test, eliminating an influence of indentation-size effects [18–20]. The values of NHD and Young’s modulus E were statistically averaged for each series and a whole sample’s surface in final.
The surface morphology of fresh cut-sections of the prepared alloys was additionally visualized using scanning electron microscope (SEM) with energy-dispersive X-ray spectroscopy (EDS) analyzer FEI QUANTA 3D 200i. The transmission electron microscopy studies with primary electron beam accelerated by 200 kV voltage were performed with a FEI Tecnai Osiris device.
Results and Discussion
In respect to our previous research on melt-quenched alloys in Gax(As0.40Se0.60)100−x system [8, 12, 14], the phase decomposition processes accompanied by Ga2Se3 crystallization occur at 4 at.% of Ga. Thus, glasses with no more than 3 at.% of Ga were suggested to be successfully used for further RE doping . The results of nanoindentation mapping presented on Fig. 2 confirm the homogeneity in these ChG via NHD and Young’s modulus E measurements. With Ga content, both of these parameters show eventual growing tendency as it is character for other homogeneous glassy alloys affected by dopants which increase density.
It is known that structural evolution in glassy As40Se60 at small amount of Ga added  is preferentially governed by appearance of As2Se4/2 blocks based on homonuclear As–As covalent chemical bonds in a glassy network, which overbalance Ga-centered polyhedral units (GaSe4/2 tetrahedrons). Such processes occur under growing input of atomic-deficient volumes contributing from bond-free solid angles around neighboring Se atoms terminated As2Se4/2 fragments. This void agglomeration trend is quickly saturated with Ga additions in ChG, thus facilitating mechanical freedom for gathering of Ga-based units. The partially decomposed Ga4(As0.40Se0.60)96 alloy display an obvious increase of scattering in the NHD (Fig. 2) and Young’s modulus E (Fig. 3) values. The drastic changes in the nanoindentation mapping are character for higher Ga content, just in Ga5(As0.40Se0.60)95 alloy. Both the NHD and E parameters are essentially bifurcated in multiple measuring series of indentation testing. The down level of bifurcation is more or less tightly grouped around some averaged values (NHD = 2.36 GPa and E = 19.5 GPa), which are very close to those observed in As40Se60 glass, while the upper level is more roughly shifted, especially for Young’s modulus E. Noteworthy, with activation of crystallization in Ga4(As0.40Se0.60)96 and Ga5(As0.40Se0.60)95 alloys, the character of free-volume void evolution is drastically changed, and now void fragmentation prevails due to stabilizing relaxation of growing Ga2Se3 crystallites .
The surface morphology of fresh cut-sections of these alloys were visualized with the help of electron microscopy to identify the appeared Ga2Se3 crystallites.
In Ga4(As0.40Se0.60)96 alloy, these crystallites represent an agglomeration of tightly connected separate pieces extended over 200–300 nm (see Fig. 4a). The EDS spectroscopy performed in scattered electrons of all constituting elements (Fig. 4b–d) allows reliable identification of crystallites composition, i.e., Ga2Se3 which is in excellent respect to the XRD data [8, 14]. Such crystallites cannot essentially affect nanoindentation mapping over a whole sample’s surface because of comparative sizes with indenter imprints, but they eventually enhance scattering in the NHD and Young’s modulus E values.
In contrast, the Ga2Se3 crystallites in Ga5(As0.40Se0.60)95 alloy get grown to larger μm sizes (Fig. 5). Under nearly uniform random distribution of such flower-like Ga2Se3 crystallite agglomerates (as it shown in Fig. 5), they left large spaces of ChG in a homogeneous glassy state. Of course, this glass is slightly enriched on As, but still close to undoped stoichiometric As2Se3. As a result, the bifurcation effect is observed in nanoindentation mapping, giving two groups of NHD and Young’s modulus E data.
Mapping of nanoscale inhomogeneities in Ga-modified As2Se3 glassy alloy was utilized exploring possibilities of conventional nanoindentation technique equipped with a Berkovitch-type diamond tip. Structural inhomogeneities were detected in Gax(As0.40Se0.60)100−x alloys having more than 3 at.% of Ga. The appearance of Ga2Se3 nanocrystallites was separately visualized in Ga-modified arsenic selenide glass using scanning and transmission electron microscopy. The Ga additions are shown to increase nanohardness and Young’s modulus of glasses, this effect attaining an obvious bifurcation trend in crystallization-decomposed Ga5(As0.40Se0.60)95 alloy.
Energy-dispersive X-ray spectroscopy
Scanning electron microscope
Adam JL, Zhang X (2014) Chalcogenide glasses: preparation, properties and applications. Woodhead Publishing, Oxford, Cambridge, New Dehli
Cui S, Chahal R, Shpotyuk Y, Boussard-Pledel C, Lucas J, Charpentier F, Tariel H, Loreal O, Nazabal V, Sire O, Monbet V, Yang Z, Lucas P, Bureau B (2014) Selenide and telluride glasses for mid-infrared bio-sensing. Proc SPIE 8938:893805
Sanghera JS, Aggarwal ID (1999) Active and passive chalcogenide glass optical fibers for IR applications: a review. J Non-Cryst Solids 256-257:6–16
Eggleton BJ, Luther-Davies B, Richardson K (2011) Chalcogenide photonics. Nat Photon 5:141–8
Troles J, Coulombier Q, Canat G, Duhant M, Renard W, Toupin P, Calvez L, Renversez G, Smektala F, El Amraoui M, Adam JL, Chartier T, Mechin D, Brilland L (2010) Low loss microstructured chalcogenide fibers for large non linear effects at 1995 nm. Opt Express 18:26647–54
Starecki F, Charpentier F, Doualan JL, Quetel L, Michel K, Chahal R, Troles J, Bureau B, Braud A, Camy P, Moizan V, Nazabal V (2015) Mid-IR optical sensor for CO2 detection based on fluorescence absorbance of Dy3+:Ga5Ge20Sb10S65 fibers. Sens Actuators B 207:518–25
Lezal D (2003) Chalcogenide glasses - survey and progress. J Optoelectron Adv Mater 5:23–34
Shpotyuk Y, Boussard-Pledel C, Nazabal V, Chahal R, Ari J, Pavlyk B, Cebulski J, Doualan JL, Bureau B (2015) Ga-modified As2Se3-Te glasses for active applications in IR photonics. Opt Mater 46:228–32
Aitken BG, Ponader CW, Quimby S (2002) Clustering of rare earths in GeAs sulfide glass. CR Chimie 5:865–72
Choi YG (2007) Spatial distribution of rare-earth ions in Se-based chalcogenide glasses with or without Ga. J Non-Cryst Solids 353:1930–5
Shpotyuk Y, Bureau B, Boussard C, Nazabal V, Golovchak R, Demchenko P, Polovynko I (2014) Effect of Ga incorporation in the As30Se50Te20 glass. J Non-Cryst Solids 398-399:19–25
Golovchak R, Shpotyuk Y, Nazabal V, Boussard-Pledel C, Bureau B, Cebulski J, Jain H (2015) Study of Ga incorporation in glassy arsenic selenides by high-resolution XPS and EXAFS. J Chem Phys 142:184501
Golovchak R, Shpotyuk Y, Thomas CM, Nazabal V, Boussard-Pledel C, Bureau B, Jain H (2015) Peculiarities of Ga and Te incorporation in glassy arsenic selenides. J Non-Cryst Solids 429:104–11
Shpotyuk Y, Ingram A, Shpotyuk O, Dziedzic A, Boussard-Pledel C, Bureau B (2016) Free-volume nanostructurization in Ga-modified As2Se3 glass. Nanoscale Res Lett 11:20
Liu C, Tang G, Luo L, Chen W (2009) Phase separation inducing controlled crystallization of GeSe2-Ga2Se3-CsCl glasses for fabricating infrared transmitting glass-ceramics. J Am Ceram Soc 92:245–8
Andrikopoulos KS, Arvanitidis J, Dracopoulos V, Christofilos D, Wagner T, Yannopoulos SN (2011) Nanoindentation and Raman studies of phase-separated Ag-As-S glasses. Appl Phys Lett 99:171911
Oliver WC, Pharr GM (1992) An improved technique for determining hardness and elastic modulus using load and displacement sensing indentation experiments. J Mater Res 7:1564–83
Li X, Bhushan B (2002) A review of nanoindentation continuous stiffness measurement technique and its applications. Mater Charact 48:11–36
Lucca DA, Herrmann K, Klopfstein MJ (2010) Nanoindentation: measuring methods and applications. CIRP Ann Manuf Technol 59:803–19
Pharr GM, Herbert EG, Gao Y (2010) The indentation size effect: a critical examination of experimental observations and mechanistic interpretations. Annu Rev Mater Res 40:271–92
This work was partly supported by Ministry of Education and Science of Ukraine under the governmental program for supporting the research projects performed by young scientists for years 2016–2018.
YS initiated the research, performed the synthesis of the tested objects, and drafted the manuscript. YS, JC, and WB designed the experimental strategy. SA, JS, and YS performed the nanoindentation measurements and data analysis. AD and WB performed the TEM, SEM, and EDS analysis. JC gave some advices on the work. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
About this article
Cite this article
Shpotyuk, Y., Adamiak, S., Dziedzic, A. et al. Nanoscale Inhomogeneities Mapping in Ga-Modified Arsenic Selenide Glasses. Nanoscale Res Lett 12, 88 (2017). https://doi.org/10.1186/s11671-017-1887-1
- Arsenic selenide glass
- Phase separation